Research Article www.acsami.org
Cite This: ACS Appl. Mater. Interfaces 2019, 11, 21645−21654
High Thermoelectric Performance in n‑Type Polycrystalline SnSe via Dual Incorporation of Cl and PbSe and Dense Nanostructures Joonil Cha,†,‡ Chongjian Zhou,†,‡ Yong Kyu Lee,†,‡ Sung-Pyo Cho,§ and In Chung*,†,‡ †
Center for Nanoparticle Research, Institute for Basic Science (IBS), Seoul 08826, Republic of Korea School of Chemical and Biological Engineering, Institute of Engineering Research and §National Center for Inter-University Research Facilities, Seoul National University, Seoul 08826, Republic of Korea
Downloaded via MOUNT ALLISON UNIV on August 6, 2019 at 09:59:11 (UTC). See https://pubs.acs.org/sharingguidelines for options on how to legitimately share published articles.
S Supporting Information *
ABSTRACT: Despite extensive studies on emerging thermoelectric material SnSe, its n-type form is largely underdeveloped mainly due to the diﬃculty in stabilizing the carrier concentration at the optimal level. Here, we dually introduce Cl and PbSe to induce n-type conduction in intrinsic p-type SnSe. PbSe alloying enhances the power factor and suppresses lattice thermal conductivity at the same time, giving a highest thermoelectric ﬁgure of merit ZT of 1.2 at 823 K for n-type polycrystalline SnSe materials. The best composition is Sn0.90Pb0.15Se0.95Cl0.05. Samples prepared by the solid-state reaction show a high maximum ZT (ZTmax) ∼1.1 and ∼0.8 parallel and perpendicular to the press direction of spark plasma sintering, respectively. Remarkably, post-ball milling and annealing processes considerably reduce structural anisotropy, thereby leading to a ZTmax ∼1.2 along both the directions. Hence, the direction giving a ZTmax is controllable for this system using the specialized preparation methods for specimens. Spherical aberration-corrected scanning transmission electron microscopic analyses reveal the presence of heavily dense edge dislocations and strain ﬁelds, not observed in the p-type counterparts, which contribute to decreasing lattice thermal conductivity. Our theoretical calculations employing a Callaway−Debye model support the experimental results for thermal transport and microscopic structures. KEYWORDS: thermoelectrics, polycrystalline SnSe, n-type, nanostructure, dual-doping
PbTe has served as a representative TE material operating in the intermediate temperature range (600−900 K) over the past 60 years.20−25 For example, a 2% Na-doped PbTe−8% SrTe system exhibits a ZT of ∼2.5 at 923 K.26 The prototype PbTebased TE modules exhibit a high power conversion eﬃciency of ∼12%.27 However, because the abundance of Te in the earth’s crust is similar to Pt, the focus of thermoelectric research has shifted toward the discovery of alternative materials consisting of earth-abundant elements while performing comparably. Although Se is 50-fold more abundant than Te and Sn is a nontoxic congener of Pb, their simple binary compound SnSe has been historically neglected for TE applications because of its apparent high electrical resistivity. In recent years, record high ZT values larger than 2.6 at 773− 923 K have been discovered for single crystal samples of pristine and doped SnSe.28,29 This extraordinarily high TE performance is mainly attributed to unique anisotropic crystal chemistry of SnSe. However, SnSe single crystals are arguably inappropriate for mass production and broad-based applications of TE technology because of high cost as well as mechanical instability and poor machinability by its layered structure. As a result, it has been of prime interest in the TE
The rapid growth of the global population causes a dramatic escalation in energy demand. Meanwhile, environmental problems ask to reduce the use of traditional fossil fuels and to develop sustainable and environmentally friendly alternative energy resources. In fact, fossil fuels are a major resource to obtain electricity and approximately two-third of them are being discarded as waste heat. Hence, recovery of this huge energy loss can concurrently contribute to solving the global energy crisis and environmental problems by enhancing energy eﬃciency and reducing the evolution of greenhouse gases.1,2 Thermoelectric (TE) technology is a good candidate for these purposes because it directly converts heat into electric energy without releasing undesirable gaseous chemical residues such as CO2 and NOx. TE power generators are mechanically reliable and environmentally stable electronic devices, operating without mechanical vibration and noise. The main interest in this technology is improving TE conversion performance for broader applications.3−16 The capability of TE materials is typically evaluated by a dimensionless ﬁgure of merit ZT = σS2T/(κele + κlat), where σ is the electrical conductivity, S is the Seebeck coeﬃcient, the product σS2 is the power factor (PF), κele and κlat are the electrical and lattice thermal conductivity, respectively, and T is the absolute temperature.17−19 © 2019 American Chemical Society
Received: May 9, 2019 Accepted: May 28, 2019 Published: May 28, 2019 21645
DOI: 10.1021/acsami.9b08108 ACS Appl. Mater. Interfaces 2019, 11, 21645−21654
ACS Applied Materials & Interfaces
SnSe materials have been reported to show highly anisotropic TE properties due to the characteristic layered structure and thereby highly ordered texture in specimens. For example, ptype Sn1−xPbxSe doped with 1% Na shows a ZTmax of ∼1.2 and 0.8 at 773 K perpendicular and parallel to the consolidating press direction, respectively.30 N-type Sn1−xPbxSe incorporated with Br exhibits the reversed trend of ZTmax of ∼0.7 and 1.2 at 823 K along the same directions as the former, respectively.40 Nanostructures in n-type polycrystalline SnSe materials have been scarcely studied despite their substantial inﬂuence on TE properties. We employed a spherical aberration-corrected scanning transmission electron microscope (Cs-corrected STEM) t o unders tand the crystal st ructure of Sn0.90Pb0.15Se0.95Cl0.05 at the atomic level and their eﬀect on TE properties. In contrast to the p-type counterparts,30,31 it contains highly dense edge dislocations and strain ﬁelds that can signiﬁcantly reduce lattice thermal conductivity.
community to develop polycrystalline SnSe materials with comparable TE performance to the single crystals. Polycrystalline SnSe has signiﬁcantly underperformed single crystal samples mainly due to the apparently larger κlat than latter.30−35 It is highly unusual in that the former has additional phonon scattering mechanisms. Recently, the origin of the paradoxically high κlat in polycrystalline SnSe was uncovered to be surface tin oxides on SnSe powder.35 It can be eﬀectively removed by the oxide removing strategy employing the chemical reduction process, leading to an exceptionally low κlat ∼0.11 W m−1 K−1 and ZT ∼2.5 for p-type polycrystalline SnSe. In contrast to the advance in p-type polycrystalline SnSe materials, the n-type counterparts have been largely underdeveloped. Only several literature studies were published and they exhibit much inferior performances to the p-type cousins.36−40 The main reason is diﬃculty in stabilizing an n-type charge carrier at the optimal level because of a substantial amount of inherent Sn vacancies and ubiquitous Sn4+ defects, making SnSe intrinsic p-type semiconductor. Just a few n-type dopants have been reported to be eﬀective for SnSe. For example, I2 coupled with S, Br, BiCl3, and PbBr2 improve ZTs of SnSe ranging from ∼0.5 to ∼1.3.36−39 Because TE devices should consist of both n- and p-type semiconductors, the underperforming type of the couple limits the overall device eﬃciency.27,41,42 Consequently, it is essential to fundamentally understand how to stabilize n-type SnSe and further enhance their TE properties. Here, we report new highly eﬃcient polycrystalline n-type SnSe materials by dually incorporating the high extent of PbSe and Cl. They synergistically contribute to improving charge transport and reducing thermal conductivity concurrently. We address a strong preference to the p-type conduction of SnSebased materials employing the multiple processes as follows. We ﬁrst synthesized a series of SnSe1−yCly (y = 0−0.08). An apparent n-type dopant Cl stabilizes the n-type conduction for samples with y larger than 0.02. Despite maximum ZT (ZTmax) of ∼0.8 obtained for the sample with y = 0.05, the electron concentration (nH) is still low at ∼4.5 × 1018 cm−3 for TE power generation and the resulting electrical conductivity (σ) is too poor. Then, we introduced excess Sn to ﬁll ubiquitous Sn vacancies in the SnSe structure, obtaining a series of Sn1+zSe0.95Cl0.05 (z = 0−0.10). As a result, nH increases moderately to ∼1.0 × 1019 cm−3 and ZTmax of ∼0.9 is achieved with the optimal excess Sn level of 0.05. Finally, we alloyed PbSe to further optimize nH for n-type SnSe. Replacing Sn by Pb can suppress the generation of intrinsic Sn vacancies because Pb almost exclusively adopts the formal charge of 2+. PbSe alloying concurrently enhances charge transport and reduces lattice thermal conductivity, leading to high ZT values for n-type SnSe. Importantly, despite the high anisotropic structure of SnSe, we are able to attain a comparable ZTmax ∼1.2 for n-type SnSe both parallel and perpendicular to the press direction of spark plasma sintering (SPS) using the dedicated preparation methods. That is, ZTmax ∼1.1 is achieved along the parallel direction of SPS for samples synthesized by the hightemperature solid-state reaction. When the samples are further processed by ball-milling and post-annealing, their thermoelectric properties become much more isotropic, exhibiting a ZTmax ∼1.2 along both the directions of SPS. This achievement is highly important in mass production and facile processability of TE materials. In fact, both p- and n-type polycrystalline
Reagents. The reagents employed in this work were used as obtained unless noted otherwise: Sn chunk (99.999%, American Elements), Se shot (99.999%, 5N Plus, Canada), anhydrous SnCl2 powder (99.99%, Sigma-Aldrich), and Pb wire (99.99%, 5N Plus, Canada). Synthesis. The synthesis of cation-excess “Sn1.05−xPbxSe0.95Cl0.05” (x = 0, 0.05, 0.10, 0.15, 0.20) ingots was achieved by reacting an appropriate ratio of starting reagents in 13 mm carbon-coated, evacuated fused-silica tubes (∼10−4 Torr) at 1223 K for 6 h, followed by quenching to water. Afterward, we will use the nominal composition for specimens. The obtained ingots were ground into powder, sieved to 2 in Phase-Separated PbTe0.7S0.3. Nat. Commun. 2014, 5, No. 4515. (22) He, J.; Zhao, L.-D.; Zheng, J.-C.; Doak, J. W.; Wu, H.; Wang, H.-Q.; Lee, Y.; Wolverton, C.; Kanatzidis, M. G.; Dravid, V. P. Role of Sodium Doping in Lead Chalcogenide Thermoelectrics. J. Am. Chem. Soc. 2013, 135, 4624−4627. (23) Biswas, K.; He, J.; Zhang, Q.; Wang, G.; Uher, C.; Dravid, V. P.; Kanatzidis, M. G. Strained Endotaxial Nanostructures with High Thermoelectric Figure of Merit. Nat. Chem. 2011, 3, 160−166. (24) Hsu, K. F.; Loo, S.; Guo, F.; Chen, W.; Dyck, J. S.; Uher, C.; Hogan, T.; Polychroniadis, E. K.; Kanatzidis, M. G. Cubic AgPbmSbTe2+m: Bulk Thermoelectric Materials with High Figure of Merit. Science 2004, 303, 818−821. (25) Pei, Y.; Shi, X.; LaLonde, A.; Wang, H.; Chen, L.; Snyder, G. J. Convergence of Electronic Bands for High Performance Bulk Thermoelectrics. Nature 2011, 473, 66−69. (26) Tan, G. J.; Shi, F. Y.; Hao, S. Q.; Zhao, L. D.; Chi, H.; Zhang, X. M.; Uher, C.; Wolverton, C.; Dravid, V. P.; Kanatzidis, M. G. Nonequilibrium Processing Leads to Record High Thermoelectric Figure of Merit in PbTe-SrTe. Nat. Commun. 2016, 7, No. 12167. (27) Jood, P.; Ohta, M.; Yamamoto, A.; Kanatzidis, M. G. Excessively Doped PbTe with Ge-Induced Nanostructures Enables High-Efficiency Thermoelectric Modules. Joule 2018, 2, 1339−1355. (28) Zhao, L. D.; Lo, S. H.; Zhang, Y. S.; Sun, H.; Tan, G. J.; Uher, C.; Wolverton, C.; Dravid, V. P.; Kanatzidis, M. G. Ultralow Thermal Conductivity and High Thermoelectric Figure of Merit in SnSe Crystals. Nature 2014, 508, 373. (29) Chang, C.; Wu, M.; He, D.; Pei, Y.; Wu, C.-F.; Wu, X.; Yu, H.; Zhu, F.; Wang, K.; Chen, Y.; Huang, L.; Li, J.-F.; He, J.; Zhao, L.-D. 3D Charge and 2D Phonon Transports Leading to High Out-of-plane ZT in n-Type SnSe Crystals. Science 2018, 360, 778−783. (30) Lee, Y. K.; Ahn, K.; Cha, J.; Zhou, C.; Kim, H. S.; Choi, G.; Chae, S. I.; Park, J.-H.; Cho, S.-P.; Park, S. H.; Sung, Y.-E.; Lee, W. B.; Hyeon, T.; Chung, I. Enhancing p-Type Thermoelectric Performances of Polycrystalline SnSe via Tuning Phase Transition Temperature. J. Am. Chem. Soc. 2017, 139, 10887−10896. (31) Ge, Z. H.; Song, D.; Chong, X.; Zheng, F.; Jin, L.; Qian, X.; Zheng, L.; Dunin-Borkowski, R. E.; Qin, P.; Feng, J.; Zhao, L. D. Boosting the Thermoelectric Performance of (Na,K)-Codoped Polycrystalline SnSe by Synergistic Tailoring of the Band Structure and Atomic-Scale Defect Phonon Scattering. J. Am. Chem. Soc. 2017, 139, 9714−9720. (32) Zhao, L. D.; Tan, G.; Hao, S.; He, J.; Pei, Y.; Chi, H.; Wang, H.; Gong, S.; Xu, H.; Dravid, V. P.; Uher, C.; Snyder, G. J.; Wolverton, C.; Kanatzidis, M. G. Ultrahigh Power Factor and Thermoelectric Performance in Hole-Doped Single-Crystal SnSe. Science 2016, 351, 141−144. (33) Wei, T. R.; Tan, G.; Zhang, X.; Wu, C. F.; Li, J. F.; Dravid, V. P.; Snyder, G. J.; Kanatzidis, M. G. Distinct Impact of Alkali-Ion Doping on Electrical Transport Properties of Thermoelectric p-Type Polycrystalline SnSe. J. Am. Chem. Soc. 2016, 138, 8875−8882. (34) Wei, T.-R.; Tan, G.; Wu, C.-F.; Chang, C.; Zhao, L.-D.; Li, J.F.; Snyder, G. J.; Kanatzidis, M. G. Thermoelectric Transport Properties of Polycrystalline SnSe Alloyed with PbSe. Appl. Phys. Lett. 2017, 110, No. 053901. (35) Lee, Y. K.; Luo, Z.; Cho, S.-P.; Kanatzidis, M. G.; Chung, I. Surface Oxide Removal for Polycrystalline SnSe Reveals Near-SingleCrystal Thermoelectric Performance. Joule 2019, 3, 719−731. (36) Zhang, Q.; Chere, E. K.; Sun, J.; Cao, F.; Dahal, K.; Chen, S.; Chen, G.; Ren, Z. Studies on Thermoelectric Properties of n-Type Polycrystalline SnSe1‑xSx by Iodine Doping. Adv. Energy Mater. 2015, 5, No. 1500360.
(1) Gingerich, D. B.; Mauter, M. S. Quantity, Quality, and Availability of Waste Heat from United States Thermal Power Generation. Environ. Sci. Technol. 2015, 49, 8297−8306. (2) Johnson, I.; Choate, W. T.; Davidson, A. Waste Heat Recovery: Technology and Opportunities in US Industry; U.S. Department of Energy Industrial Technologies Program, 2008. (3) Banik, A.; Shenoy, U. S.; Saha, S.; Waghmare, U. V.; Biswas, K. High Power Factor and Enhanced Thermoelectric Performance of SnTe-AgInTe2: Synergistic Effect of Resonance Level and Valence Band Convergence. J. Am. Chem. Soc. 2016, 138, 13068−13075. (4) Tan, G.; Zhao, L.-D.; Kanatzidis, M. G. Rationally Designing High-Performance Bulk Thermoelectric Materials. Chem. Rev. 2016, 116, 12123−12149. (5) Kleinke, H. New bulk Materials for Thermoelectric Power Generation: Clathrates and Complex Antimonides. Chem. Mater. 2010, 22, 604−611. (6) Guo, Q.; Chan, M.; Kuropatwa, B. A.; Kleinke, H. Enhanced Thermoelectric Properties of Variants of Tl9SbTe6 and Tl9BiTe6. Chem. Mater. 2013, 25, 4097−4104. (7) Rogl, G.; Grytsiv, A.; Rogl, P.; Peranio, N.; Bauer, E.; Zehetbauer, M.; Eibl, O. n-Type Skutterudites (R,Ba,Yb)yCo4Sb12 (R = Sr, La, Mm, DD, SrMm, SrDD) Approaching ZT≈2.0. Acta Mater. 2014, 63, 30−43. (8) Choi, G.; Kim, H. S.; Lee, K.; Park, S. H.; Cha, J.; Chung, I.; Lee, W. B. Study on Thermal Conductivity and Electrical Resistivity of AlCu Alloys Obtained by Boltzmann Transport Equation and firstprinciples simulation: Semi-empirical approach. J. Alloys. Compd. 2017, 727, 1237−1242. (9) Shuai, J.; Ge, B.; Mao, J.; Song, S.; Wang, Y.; Ren, Z. Significant Role of Mg Stoichiometry in Designing High Thermoelectric Performance for Mg3(Sb,Bi)2-Based n-Type Zintls. J. Am. Chem. Soc. 2018, 140, 1910−1915. (10) Jana, M. K.; Pal, K.; Warankar, A.; Mandal, P.; Waghmare, U. V.; Biswas, K. Intrinsic Rattler-Induced Low Thermal Conductivity in Zintl Type TlInTe2. J. Am. Chem. Soc. 2017, 139, 4350−4353. (11) Hu, Y.; Chen, C.-W.; Cao, H.; Makhmudov, F.; Grebenkemper, J. H.; Abdusalyamova, M. N.; Morosan, E.; Kauzlarich, S. M. Tuning Magnetism of [MnSb4]9− Cluster in Yb14MnSb11 through Chemical Substitutions on Yb Sites: Appearance and Disappearance of Spin Reorientation. J. Am. Chem. Soc. 2016, 138, 12422−12431. (12) Liu, Y.; Sahoo, P.; Makongo, J. P. A.; Zhou, X.; Kim, S.-J.; Chi, H.; Uher, C.; Pan, X.; Poudeu, P. F. P. Large Enhancements of Thermopower and Carrier Mobility in Quantum Dot Engineered Bulk Semiconductors. J. Am. Chem. Soc. 2013, 135, 7486−7495. (13) Kim, H.; Kaviany, M.; Thomas, J. C.; Van der Ven, A.; Uher, C.; Huang, B. Structural Order-Disorder Transitions and Phonon Conductivity of Partially Filled Skutterudites. Phys. Rev. Lett. 2010, 105, No. 265901. (14) Zhou, C.; Lee, Y. K.; Cha, J.; Yoo, B.; Cho, S.-P.; Hyeon, T.; Chung, I. Defect Engineering for High-Performance n-Type PbSe Thermoelectrics. J. Am. Chem. Soc. 2018, 140, 9282−9290. (15) Zhou, C.; Yu, Y.; Lee, Y. K.; Cojocaru-Mirédin, O.; Yoo, B.; Cho, S.-P.; Im, J.; Wuttig, M.; Hyeon, T.; Chung, I. HighPerformance n-Type PbSe−Cu2Se Thermoelectrics through Conduction Band Engineering and Phonon Softening. J. Am. Chem. Soc. 2018, 140, 15535−15545. (16) Park, K.; Ahn, K.; Cha, J.; Lee, S.; Chae, S. I.; Cho, S.-P.; Ryee, S.; Im, J.; Lee, J.; Park, S.-D.; Han, M. J.; Chung, I.; Hyeon, T. Extraordinary Off-Stoichiometric Bismuth Telluride for Enhanced nType Thermoelectric Power Factor. J. Am. Chem. Soc. 2016, 138, 14458−14468. (17) Sootsman, J. R.; Chung, D. Y.; Kanatzidis, M. G. New and Old Concepts in Thermoelectric Materials. Angew. Chem., Int. Ed. 2009, 48, 8616−8639. (18) Kanatzidis, M. G. Discovery-Synthesis, Design, and Prediction of Chalcogenide Phases. Inorg. Chem. 2017, 56, 3158−3173. (19) Kanatzidis, M. G. Nanostructured Thermoelectrics: The New Paradigm? Chem. Mater. 2010, 22, 648−659. 21653
DOI: 10.1021/acsami.9b08108 ACS Appl. Mater. Interfaces 2019, 11, 21645−21654
ACS Applied Materials & Interfaces (37) Wang, X.; Xu, J.; Liu, G.; Fu, Y.; Liu, Z.; Tan, X.; Shao, H.; Jiang, H.; Tan, T.; Jiang, J. Optimization of Thermoelectric Properties in n-Type SnSe Doped with BiCl3. Appl. Phys. Lett. 2016, 108, No. 083902. (38) Li, S.; Wang, Y.; Chen, C.; Li, X.; Xue, W.; Wang, X.; Zhang, Z.; Cao, F.; Sui, J.; Liu, X.; Zhang, Q. Heavy Doping by Bromine to Improve the Thermoelectric Properties of n-type Polycrystalline SnSe. Adv. Sci. 2018, 5, No. 1800598. (39) Li, D.; Tan, X.; Xu, J.; Liu, G.; Jin, M.; Shao, H.; Huang, H.; Zhang, J.; Jiang, J. Enhanced Thermoelectric Performance in n-Type Polycrystalline SnSe by PbBr2 Doping. RSC Adv. 2017, 7, 17906− 17912. (40) Chang, C.; Tan, Q.; Pei, Y.; Xiao, Y.; Zhang, X.; Chen, Y.-X.; Zheng, L.; Gong, S.; Li, J.-F.; He, J.; Zhao, L.-D. Raising Thermoelectric Performance of n-Type SnSe via Br Doping and Pb Alloying. RSC Adv. 2016, 6, 98216−98220. (41) Park, S. H.; Jin, Y.; Cha, J.; Hong, K.; Kim, Y.; Yoon, H.; Yoo, C.-Y.; Chung, I. High-Power-Density Skutterudite-Based Thermoelectric Modules with Ultralow Contact Resistivity Using Fe−Ni Metallization Layers. ACS Appl. Energy Mater. 2018, 1, 1603−1611. (42) Salvador, J. R.; Cho, J. Y.; Ye, Z.; Moczygemba, J. E.; Thompson, A. J.; Sharp, J. W.; Koenig, J. D.; Maloney, R.; Thompson, T.; Sakamoto, J.; Wang, H.; Wereszczak, A. A. Conversion Efficiency of Skutterudite-Based Thermoelectric Modules. Phys. Chem. Chem. Phys. 2014, 16, 12510−12520. (43) Hÿtch, M. J.; Snoeck, E.; Kilaas, R. Quantitative Measurement of Displacement and Strain Fields from HREM Micrographs. Ultramicroscopy 1998, 74, 131−146. (44) Lotgering, F. K. Topotactical Reactions with Ferrimagnetic Oxides Having Hexagonal Crystal StructuresI. J. Inorg. Nucl. Chem. 1959, 9, 113−123. (45) Wang, X.; Xu, J.; Liu, G.-Q.; Tan, X.; Li, D.; Shao, H.; Tan, T.; Jiang, J. Texturing Degree Boosts Thermoelectric Performance of Silver-Doped Polycrystalline SnSe. NPG Asia Mater. 2017, 9, No. e426. (46) Fu, Y.; Xu, J.; Liu, G.-Q.; Tan, X.; Liu, Z.; Wang, X.; Shao, H.; Jiang, H.; Liang, B.; Jiang, J. Study on Thermoelectric Properties of Polycrystalline SnSe by Ge Doping. J. Electron. Mater. 2017, 46, 3182−3186. (47) Li, Y.; Shi, X.; Ren, D.; Chen, J.; Chen, L. Investigation of the Anisotropic Thermoelectric Properties of Oriented Polycrystalline SnSe. Energies 2015, 8, 6275. (48) Villars, P.; Prince, A.; Okamoto, H. Handbook of Ternary Alloy Phase Diagrams; ASM International, 1995. (49) Woolley, J. C.; Berolo, O. Phase Studies of the Pb1−xSnxSe Alloys. Mater. Res. Bull. 1968, 3, 445−450. (50) Volykhov, A. A.; Shtanov, V. I.; Yashina, L. V. Phase Relations between Germanium, Tin, and Lead Chalcogenides in Pseudobinary Systems Containing Orthorhombic Phases. Inorg. Mater. 2008, 44, 345−356. (51) Su, D.; Zhu, Y. Scanning Moiré Fringe Imaging by Scanning Transmission Electron Microscopy. Ultramicroscopy 2010, 110, 229− 233. (52) Xin, J.; Wu, H.; Liu, X.; Zhu, T.; Yu, G.; Zhao, X. Mg Vacancy and Dislocation Strains as Strong Phonon Scatterers in Mg2Si1−xSbx Thermoelectric Materials. Nat. Energy 2017, 34, 428−436. (53) Yang, L.; Chen, Z.-G.; Hong, M.; Wang, L.; Kong, D.; Huang, L.; Han, G.; Zou, Y.; Dargusch, M.; Zou, J. n-Type Bi-doped PbTe Nanocubes with Enhanced Thermoelectric Performance. Nat. Energy 2017, 31, 105−112. (54) Chen, Z.; Ge, B.; Li, W.; Lin, S.; Shen, J.; Chang, Y.; Hanus, R.; Snyder, G. J.; Pei, Y. Vacancy-Induced Dislocations within Grains for High-Performance PbSe Thermoelectrics. Nat. Commun. 2017, 8, No. 13828. (55) Zhou, C.; Lee, Y. K.; Cha, J.; Yoo, B.; Cho, S.-P.; Hyeon, T.; Chung, I. Defect Engineering for High-Performance n-Type PbSe Thermoelectrics. J. Am. Chem. Soc. 2018, 140, 9282−9290.
(56) Hÿtch, M. J.; Snoeck, E.; Kilaas, R. Quantitative Measurement of Displacement and Strain Fields from HREM Micrographs. Ultramicroscopy 1998, 74, 131−146. (57) Wang, Z.; Saito, M.; McKenna, K. P.; Ikuhara, Y. Polymorphism of Dislocation Core Structures at the Atomic Scale. Nat. Commun. 2014, 5, No. 3239. (58) Callaway, J.; von Baeyer, H. C. Effect of Point Imperfections on Lattice Thermal Conductivity. Phys. Rev. 1960, 120, 1149−1154. (59) Pumphrey, P. H.; Gleiter, H. The Annealing of Dislocations in High-Angle Grain Boundaries. Philos. Mag. 1974, 30, 593−602.
DOI: 10.1021/acsami.9b08108 ACS Appl. Mater. Interfaces 2019, 11, 21645−21654